Production of Pig Iron by Smelting of Blended Pre-Reduced Titaniferous Magnetite Ore and Hematite Ore Using Lean Grade Coal
The rapid depletion of high-grade iron ore (Fe2O3) has gained attention on the use of other sources of iron ore. Titaniferous magnetite ore (TMO) is a special type of magnetite ore having high titania content (23.23% TiO2 present in this case). Due to high TiO2 content and high density, TMO cannot be treated by the conventional smelting reduction. In this present work, the TMO has been collected from high-grade metamorphic terrain of the Precambrian Chotanagpur gneissic complex situated in the eastern part of India (Shaltora area, Bankura district, West Bengal) and the hematite ore has been collected from Visakhapatnam Steel Plant (VSP), Visakhapatnam. At VSP, iron ore is received from Bailadila mines, Chattisgarh of M/s. National Mineral Development Corporation. The preliminary characterization of TMO and hematite ore (HMO) has been investigated by WDXRF, XRD and FESEM analyses. Similarly, good quality of coal (mainly coking coal) is also getting depleted fast. The basic purpose of this work is to find how lean grade coal can be utilised along with TMO for smelting to produce pig iron. Lean grade coal has been characterised by using TG/DTA, proximate and ultimate analyses. The boiler grade coal has been found to contain 28.08% of fixed carbon and 28.31% of volatile matter. TMO fines (below 75 μm) and HMO fines (below 75 μm) have been separately agglomerated with lean grade coal fines (below 75 μm) in the form of briquettes using binders like bentonite and molasses. These green briquettes are dried first in oven at 423 K for 30 min and then reduced isothermally in tube furnace over the temperature range of 1323 K, 1373 K and 1423 K for 30 min & 60 min. After reduction, the reduced briquettes are characterized by XRD and FESEM analyses. The best reduced TMO and HMO samples are taken and blended in three different weight percentage ratios of 1:4, 1:8 and 1:12 of TMO:HMO. The chemical analysis of three blended samples is carried out and degree of metallisation of iron is found to contain 89.38%, 92.12% and 93.12%, respectively. These three blended samples are briquetted using binder like bentonite and lime. Thereafter these blended briquettes are separately smelted in raising hearth furnace at 1773 K for 30 min. The pig iron formed is characterized using XRD, microscopic analysis. It can be concluded that 90% yield of pig iron can be achieved when the blend ratio of TMO:HMO is 1:4.5. This means for 90% yield, the maximum TMO that could be used in the blend is about 18%.
Digital Object Identifier (DOI): doi.org/10.5281/zenodo.1125991Procedia APA BibTeX Chicago EndNote Harvard JSON MLA RIS XML ISO 690 PDF Downloads 1203
 G. M. Chowdhury, G. G. Roy and S. K. Roy: ‘Reduction kinetics of iron ore-graphite composite pellets in a packed-bed reactor under inert and reactive atmospheres’, Metall. Mater. Trans. B, 2008, 39, 160–178.
 Bitan Kumar Sarkar, Saikat Samanta, Rajib Dey and Gopes Chandra Das, A Study on Reduction Kinetics of Titaniferous Magnetite Ore Using Lean Grade Coal, International Journal of Mineral Processing, 152, 36–45 (2016).
 H. M. Ahmed, N. Viswanathan and B. Bjorkman: ‘Composite pellets – a potential raw material for Iron-making’, Steel Res. Int., 2014, 85, 293–306.
 R. Robinson: ‘Studies in low temperature self-reduction of by-products from integrated iron and steelmaking’, Luleå tekniska universitet, Luleå tekniska universitet, Doctoral thesis (2008), 69.
 D. Adolfsson, R. Robinson, J. Blagojevic and F. Su: ‘Assessment of ladle slag as binder alternative for cold bonded briquettes,’ Global Symposium on Recycling, Waste Treatment and Clean Technology, Cancun, Mexico, October 12–15, 2008, Minerals, Metals & Materials Society.
 S. Ueda, K. Watanabe, K. Yanagiya, R. Inoue and T. Ariyama: ‘Improvement of reactivity of carbon iron ore composite with biomass char for blast furnace’, ISIJ Int., 2009, 49, 1505–1512.
 S. Ueda, K. Yanagiya, K. Watanabe, T. Murakami, R. Inoue and T. Ariyama: ‘Reaction model and reduction behavior of carbon iron ore composite in blast furnace’, ISIJ Int., 2009, 49, 827–836.
 T. Murakami, T. Nishimura and E. Kasai: ‘Lowering reduction temperature of iron ore and carbon composite by using ores with high combined water content’, ISIJ Int., 2009, 49, 1686–1693.
 Y. Matsui, M. Sawayama, A. Kasai, Y. Yamagata and F. Noma: ‘Reduction behavior of carbon composite iron ore hot briquette in shaft furnace and scope on blast furnace performance reinforcement’, ISIJ Int., 2003, 43, 1904–1912.
 S. K. Dutta, A. Ghosh: ‘Study of nonisothermal reduction of iron ore-coal/char composite pellet’, MMTB, 1994, 25, 15–26.
 S. K. Dutta, A. Ghosh: ‘A new method for measurement of degree of reduction in composite pellets of iron ore with carbonaceous matter’, ISIJ Int., 1993, 33, 1104–1106.
 H. M. Ahmed, N. N. Viswanathan and B. Björkman, Isothermal reduction kinetics of self-reducing mixtures, Ironmaking & Steelmaking, DOI 10.1080/03019233.2016.1165497 (2016).
 R. H. Nafziger and R. R. Gordan, Prereduction and melting of domestic titaniferous materials, Metallurgical Transactions B, 1983, pp-55-62.
 V. E. Roshchin, A. V. Asanov and A. V. Roshchin, Possibilities of two-stage processing of titaniferous magnetite ore concentrates, Russian Metallurgy (Metally), 2011, pp-499-508.
 M. M. Manamela and P. C. Pistorius, Ore size does affect direct reduction of titaniferous magnetite, The Journal of the South African institute of Mining and Metallurgy, 2005, pp-183-186.
 V. E. Roshchin, A. V. Asanov and A. V. Roshchin, Solid-phase prereduction of iron-vanadium concentrates and liquid-phase separation of the products of their reduction, Russian Metallurgy (Metally), 2010, pp-1001-08.
 Tu Hu, Xuewei Lv, Chenguang Bai, Zhingang Lun and Guibao Qiu, Reduction behaviour of panzhihua titanomagnetite concentrates with coal, Metallurgical and Materials Transactions B, 2013, pp-252-260.
 R. Sah, S. K. Dutta, Kinetic studies of iron ore-coal composite pellet reduction by TG/DTA, Trans Indian Inst Met, 64 (6) (2011), 583-591.
 H. W. Gudenau, D. Senk, S. Wang, K. De Melo Martins, C. Stephany, Research in the reduction of iron ore agglomerates including coal and c-containing dust, ISIJ Internationals, 45 (2005), 603-608.
 G. Liu, V. Strezov, J. A. Lucas, L. J. Wibberley, Thermal investigations of direct iron ore reduction with coal, Thermochimica acta, 410 (2004), 133-140.
 W. Lu and D. F. Huang: ‘The evolution of ironmaking process based on coal-containing iron ore agglomerates’, ISIJ Int., 2001, 41, 807– 812.
 A. K. Vaish, R. C. Gupta, S. P. Mehrotra, Thermodynamic and kinetic aspects of the smelting reduction of multimetallic Indian magnetite ore, Journal of Metallurgy and Materials Science, 48 (2006), 1-12.